channeled polymeric scaffolds with polypeptide gel filling ... channeled polymeric scaffolds with...
Post on 26-Feb-2020
Embed Size (px)
European Polymer Journal 70 (2015) 331–341
Contents lists available at ScienceDirect
European Polymer Journal
journal homepage: www.elsevier .com/locate /europol j
Channeled polymeric scaffolds with polypeptide gel filling for lengthwise guidance of neural cells
http://dx.doi.org/10.1016/j.eurpolymj.2015.07.033 0014-3057/� 2015 Elsevier Ltd. All rights reserved.
⇑ Corresponding author. E-mail address: firstname.lastname@example.org (A. Vallés-Lluch).
1 Equal contribution.
A. Conejero-García a,1, G. Vilariño-Feltrer a,1, C. Martínez-Ramos a, M. Monleón Pradas a,b, A. Vallés-Lluch a,⇑ a Center for Biomaterials and Tissue Engineering, Universitat Politècnica de València, C. de Vera s/n, 46022 Valencia, Spain b Networking Research Center on Bioengineering, Biomaterials and Nanomedicine, Valencia, Spain
a r t i c l e i n f o
Article history: Received 25 February 2015 Received in revised form 5 July 2015 Accepted 18 July 2015 Available online 20 July 2015
Keywords: Scaffold NGF RAD16-I Neural conduct Neuroglia Axonal growth
a b s t r a c t
CNS damages are often irreversible since neurons of the central nervous system are unable to regenerate after an injury. As a new strategy within the nervous system tissue engineering, multifunctional systems based on two different biomaterials to support axonal guidance in damaged connective tracts have been developed herein. These systems are composed of a channeled scaffold made of ethyl acrylate and hydroxyethyl acrylate copolymer, P(EA-co-HEA), with parallel tubular micropores, combined with an injectable and in situ gelable self-assembling polypeptide (RAD16-I) as pores filler. The polymer scaffold is intended to provide a three-dimensional context for axon growth; subsequently, its morphology and physicochemical parameters have been determined by scanning electron microscopy, density measurements and compression tests. Besides, the hydrogel acts as a cell-friendly nanoenvironment while it creates a gradient of bioactive molecules (nerve growth factor, NGF) along the scaffolds channels; the chemotactic effect of NGF has been evaluated by a quantitative ELISA assay. These multifunctional systems have shown ability to keep circulating NGF, as well as proper short-term in vitro biological response with glial cells and neural progenitors.
� 2015 Elsevier Ltd. All rights reserved.
Central nervous system (CNS) is particularly vulnerable to damages and defects like strokes or diseases, and hence medicine has traditionally made an intense effort to discover effective treatments upon investigation of their onset and symptoms. In Parkinson’s disease, e.g., an acute loss of dopaminergic neurons in the substantia nigra occurs, followed by a lack for dopamine in the striatum [1,2]. Although mechanisms are still unclear [3–5], latest discoveries improved our knowledge about where the disease begins and how this effect expands . However, all CNS damages worsen soon after their onset due to the low rate of regeneration in the nervous system. This regeneration is only effective in hippocampus and olfactory bulb, although there are evidences of neurogenesis in adult mammals in several additional areas, including striatum and substantia nigra .
Neural stem cells (NSCs) present some features such as a multipotent nature and a common cluster conformation known as proliferative neurospheres in response to defined signals; this is why neural stem cell transplantation has been considered
http://crossmark.crossref.org/dialog/?doi=10.1016/j.eurpolymj.2015.07.033&domain=pdf http://dx.doi.org/10.1016/j.eurpolymj.2015.07.033 mailto:email@example.com http://dx.doi.org/10.1016/j.eurpolymj.2015.07.033 http://www.sciencedirect.com/science/journal/00143057 http://www.elsevier.com/locate/europolj
332 A. Conejero-García et al. / European Polymer Journal 70 (2015) 331–341
as a promising strategy for the treatment of lesions [5,8]. However, the effectiveness of this therapy is limited because of the lack of support from the host damaged environment and a low cell survival rate after transplantation.
In order to stop or effectively revert the progression of disease, synthetic biomaterials have been widely tested to avoid the drawbacks of current therapies. Indeed, they are one of the cornerstones in tissue engineering, as they might support cell grafting by providing a physical three-dimensional context to lodge and protect them, maximizing thus cell transplantation efficiency [9–11]. The use of scaffolds with selected properties (topography, chemical interactions, mechanical modulus. . .) can also improve chemical cell-(protein)-biomaterial and cell–cell communication and, subsequently, cell adhesion, proliferation, migration, and differentiation [10,12].
Degradable materials are intended just as temporary supports and are thus the most employed ones; however, there is room for their opposites in this field, for example in CNS degenerative defects that are triggered or aggravated by gene-derived cues . In general, the use of non-degradable polymers is desirable when the host tissue is not able to ensure a functional recovery by itself, and supply a long-term support in terms of three-dimensional innocuous protective environment. For instance, elastomeric polymers, like those made of ethyl acrylate (EA), or their copolymers with hydroxyethyl acrylate (HEA), can also interact with cell integrins and other membrane receptors via adsorbed proteins to modulate cell response, due to their paired hydrophobic–hydrophilic domains. Namely, P(EA-co-HEA) 90/10 w/w scaffolds have previously demonstrated good biocompatibility in in vitro and in vivo studies, allowing cells to adhere, migrate and differentiate [14–17].
Likewise, extracellular matrix-like hydrogels such as RAD16-I, in spite of being difficult to handle, have widespread experimental and clinical applications, including cell culture, drug delivery and regeneration of CNS tissue, cardiac tissue or cartilage and bone growth [18–22], and such an edge has to be considered to mimic realistically a complex tissue-like structure.
To fully make the most of the tissue engineering potential, in recent years numerous bioactive stimuli such as neu- rotrophic factors, electromagnetic fields and extracellular matrix molecules have been used to fill the short-term deficiencies in the site of injury, together with biomaterials. Bioactive nerve growth factor (NGF), brain-derived neurotrophic factor (BDNF), fibroblast growth factor (FGF) and glial growth factor (GDNF) are some of the most extensively molecules explored as treatments for CNS injuries [23–25]. In particular, NGF has also been tested with different delivery systems using fibrin, gelatin or other polymers, leading to an improvement of axon extension of neural cells [26,27].
Acrylate spongy or grid-like scaffolds have been combined with RAD16-I gel and their biological performance has already been studied in vitro and in vivo [14,28–31]. Notwithstanding, the microarchitecture of scaffolds herein used is particular, in the sense that channels are smaller in diameter, lengthwise oriented and not connected between them; these features make them potential candidates for dentin regeneration, which has been the case in [32,33] and for neural regeneration . In this work, the in vitro biological response of P(EA-co-HEA) 90/10 scaffolds with parallel channels filled with a self-assembling polypeptide (RAD16-I) has been evaluated to select the material substrate, in terms of how crucial the chan- nels diameter is to attain guided axon extension and the potential interest of incorporating the RAD16-I filler to improve cell proliferation and migration. The gel allows the diffusion of chemicals from one edge to the other, together with the coloniza- tion by cells seeded up there. Thus, it has been assessed whether the chemotaxis of NGF on a co-culture of Schwann cells and neurospheres along the scaffold channels improves axon regeneration, besides neural cell survival, proliferation and differentiation.
2. Materials and methods
2.1. Reagents and materials
Reagents were purchased from Sigma–Aldrich, except the N-N-dimethylformamide (Scharlab). Schwann cells and culture media were purchased from Innoprot, MTS assay kit from Promega, and putrescine, progesterone, sodium selenite, apo-t-transferrin, insulin, paraformaldehyde, Tween-20 and BSA from Sigma–Aldrich. DMEM/F12, glucose, HEPES,
L-glutamine, penicillin/streptomycin, BDNF, FGF, StemPro acutasse, Quant-iT DNA assay, Alexa goat anti-rabbit 488 and DAPI were obtained from Life Technologies, polyclonal rabbit anti-GFAP from Dako Cytomation and NGF sandwich ELISA kit ChemiKine from Millipore.
2.2. Preparation of P(EA-co-HEA) scaffolds
P(EA-co-HEA) scaffolds were fabricated by thermal polymerization, using glass tubes (4 mm in diameter) filled with a bundle of polyacrylonitrile (PAN) fibers with two different diameters: 10 and 50 lm. The fibers were set parallels and stretched, as described in . Briefly, a monomeric solution was prepared with ethyl acrylate (EA) and hydroxyethyl acrylate (HEA), 90/10% w/w, respectively, adding ethylene glycol dimethacrylate (EGDMA; 1 wt%) as crosslinker and benzoyl peroxide (BPO; 0.5 wt%) as thermal initiator. The solution was stirred and vacuum-injected into the molds, which were sealed and cured for 24 h at 60 �C. After this first polymerization step, temperature was raised to 90 �C for 24 h more, to post-polymerize any unreacted reagents. To obtain porous scaffolds, the bulk polymeric blocks were cut into sections of 6 mm in length and rinsed in N-N-dimethylformamide (DMF) for 72 h, changing the solution every